Microbial synthesized biodegradable PHBHHxPEG hybrid copolymer as an efficient intracellular delivery nanocarrier for kinase inhibitor
© Lu et al.; licensee BioMed Central Ltd. 2014
Received: 15 August 2013
Accepted: 11 January 2014
Published: 18 January 2014
Protein Kinases are key regulators of cell function and play essential roles in the occurrence and development of many human diseases. Many kinase inhibitors have been used for molecular targeted treatment of those diseases such as cancer and inflammation. However, those highly hydrophobic kinase inhibitors shared the common features of poor bioavailability and limited in vivo half-life, which strongly impeded their practical applications. Our previous study demonstrated that microbial synthesized biodegradable polyester poly(3-hydroxybutyrate-co-3-hydroxyhexanoate) (PHBHHx), a member of polyhydroxyalkanoates (PHAs) family, could serve as a promising delivery nanocarrier for those hydrophobic kinase inhibitors. Recently, a novel natural synthesized hybrid copolymer, PEG200 end-capped PHBHHx (PHBHHxPEG) was produced by Aeromonas hydrophila fermentation. In this study, the novel PHBHHxPEG NPs were prepared and investigated to serve as intracellular delivery nanocarriers for sustained release of hydrophobic kinase inhibitors.
PHBHHxPEG nanoparticles (NPs) prepared by an emulsification–solvent evaporation method were spherical with a diameter around 200 nm. The entrapment efficiency on rapamycin in PHBHHxPEG NPs was 91.9% and the sustained release of rapamycin from PHBHHxPEG NPs could be achieved for almost 10 days. The cellular uptake of PHBHHxPEG NPs was significant higher than that of PHBHHx NPs. The anti-proliferation effect and mTOR inhibition ability of rapamycin-loaded PHBHHxPEG NPs was stronger than that of drug-loaded PHBHHx NPs and free rapamycin.
PHBHHxPEG NPs could achieve the efficient entrapment and sustained release of rapamycin. The novel biodegradable PHBHHxPEG appeared a promising nanocarrier for sustained delivery of hydrophobic kinase inhibitors with improved cellular uptake and kinase inhibition efficiency.
KeywordsPolyhydroxyalkanoate PEG Rapamycin Nanoparticle Drug delivery
Protein kinases play essential roles in signal transduction and regulation by phosphorylating other proteins to alter their enzymatic activity, cellular location, or association with other proteins. Phosphorylation of the target protein is a necessary and key step in the occurrence and development of some cancers and inflammatory diseases. Therefore, protein kinase inhibitors which specifically block the action of one or more protein kinases have been used as drugs for molecular targeted treatment of cancer and inflammatory diseases. However, poor bioavailability and limited in vivo half-life are rather common features of many kinase inhibitors that usually are highly hydrophobic compounds. For example, rapamycin (RAP, also known as Sirolimus) isolated from Streptomyces hygroscopicus is such kind of hydrophobic kinase inhibitor which has already been approved by US Food and Drug Administration (FDA) as an immunosuppressive drug to prevent the rejection of solid organ transplants . RAP is a natural inhibitor of the mammalian target of rapamycin (mTOR) which is a critical regulator of cell growth, proliferation and survival. Dysregulation of mTOR activities often occurs in a variety of human malignant diseases, making it a crucial and validated target for the cancer intervention . The anti-proliferation activity of RAP was evaluated and it was found that RAP could also inhibit the proliferation of a number of tumor cell lines . However, since it is a strongly hydrophobic compound and only slightly soluble in several acceptable excipients such as ethanol, propylene glycol and polyethylene glycol 400 , RAP is only available in oral but with a relative low bioavailability of around 17% . Therefore, conventional dosage formulations of RAP could not fulfill the demand for anti-proliferation therapy.
Biodegradable polymeric nanoparticles are more and more frequently used in drug delivery systems and represent one of the most rapidly developing areas, which have now attracted growing interest of chemists, pharmacists and biologists. Nanosized polymeric nanoparticles provide a comprehensive platform for achieving the enhanced drug solubility/stability, improving the effectiveness of drug therapy and reducing the side effects of the loaded drug to healthy tissues. Many different natural and synthetic polymers have been developed as drug delivery carriers. Polyhydroxyalkanoates (PHAs) are a family of biodegradable aliphatic polyesters which are synthesized by a wide range of bacteria. PHAs have been extensively studied as implantable tissue repair/regeneration devices and other biomedical devices such as sutures and suture fasteners, because of their good biocompatibility and biodegradability [6, 7]. Recently, PHAs have also been explored for controlled drug-release applications [8, 9]. Based on their polyester aliphatic properties, PHAs are more efficient in encapsulating the hydrophobic compounds and thus would be especially beneficial for hydrophobic drugs. Several commercialized PHAs, for example, polyhydroxybutyrate (PHB) and poly(3-hydroxybutyrate-co-3-hydroxy-hexanoate) (PHBHHx), have been successfully developed into nanoparticles and investigated for the entrapment and release profiles of hydrophobic compounds. The drug-loaded PHA nanoparticles demonstrated sustained release of hydrophobic drugs and enhanced bioavailability in cell-based assays .
In our previous studies, a novel naturally synthesized hybrid polyester, polyethylene glycol 200 (PEG200) end-capped poly(3-hydroxybutyrate-co-3- hydroxyhexanoate) (PHBHHxPEG) was directly produced by Aeromonas hydrophila fermentation . In this study, the novel PHBHHxPEG NPs were prepared and investigated to serve as the nanocarrier for sustained release of a hydrophobic kinase inhibitor like RAP. RAP cellular uptake of PHBHHxPEG NPs, in vitro release of RAP from the NPs, cellular proliferation inhibition and kinase inhibition of RAP-loaded NPs were investigated. The results obtained in this study indicated that the microbial synthesized PHBHHxPEG hybrid copolymer represents a promising material to serve as an intracellular drug delivery carrier for sustained release of hydrophobic kinase inhibitors.
Preparation and characterization of PHBHHx and PHBHHxPEG NPs
The diameters and polydispersities of the free and rapamycin/rhodamine-loaded nanoparticles
In vitro release of rapamycin
Interestingly, the release of RAP from PHA-based NPs was more efficient than that from PLA NPs. Indeed, more than 95% of the drug could be released from the PHBHHx and PHBHHxPEG NPs after 10 days. On the contrary, more than 30% RAP still remained in the PLA NPs even after 10 days, which indicated that this 30% of drug was strongly encapsulated in the PLA NPs and could not be released. Such behavior might be explained by the relativly poor crystalline nature of PHBHHx and PHBHHxPEG materials, thus allowing RAP to diffuse from the loose particle core. These results thus indicated that the PHBHHx and PHBHHxPEG nanoparticles could efficiently and effectively extend the release profile of RAP and could be eventually used as controlled delivery carriers for hydrophobic drugs.
Cellular uptake of PHBHHx and PHBHHxPEG NPs
In vitro cytotoxicity evaluation of PHBHHx and PHBHHxPEG NPs
Effects of rapamycin-loaded NPs on proliferation of PC3 cells
Effects of RAP-loaded NPs on mTOR activity
Because poor bioavailability and limited in vivo half-life are rather common features of many kinase inhibitors that usually are highly hydrophobic compounds, the development of polymer-based nanocarrier for kinase inhibitors provided a promising strategy to improve their therapeutic activity by releasing drugs in a sustained manner, and consequently enhancing their bioavailability, improving their solubility, and reducing the toxic side effects . In addition, drug-carrying nanoparticles could be passively accumulated in tumor or inflammatory tissues through the enhanced permeability and retention (EPR) effect and thus could further increase the effectual concentration of hydrophobic drugs . Polymeric nanoparticles have been extensively studied as drug carriers  and several polymer-based, nanoparticulated formulations have been approved by the FDA for clinical applications . PHAs are linear biopolyesters produced as energy- and carbon-storage materials by many bacteria. The medical applications of PHA have been extensively explored in recent years for implant biomedical applications . Several members of PHAs, such as PHB and PHBHHx, have also been developed into nanoparticles and investigated for controlled drug-release applications [8, 9, 17]. Our previous data indicated that they were efficient in encapsulating hydrophobic compounds such as the phosphoinositide-3-kinases (PI3Ks) inhibitor TGX221 (Mw = 364.4). In this study, rapamycin, a mTOR inhibitor with relative high molecular mass of 914.17, was used to investigate the entrapment and release abilities of PHA NPs for high molecular weight kinase inhibitors. Both PHBHHx and PHBHHxPEG NPs showed higher rapamycin entrapment efficiency (more than 90%) and more complete drug release than that of PLA NPs, which was consisted with the study of TGX221-loaded PHA NPs. This indicated the advantage of PHA-based NPs in the entrapment and sustained release of hydrophobic kinase inhibitors. The results of this study also showed that release of rapamycin from PHBHHxPEG NPs was faster than that from PHBHHx NPs, which might be due to the incorporation of PEG fragments and the relativly low molecular weight of PHBHHxPEG.
The incorporation of PEG could also confer more hydrophilicity to PHBHHxPEG NPs. This might explain the enhanced cellular uptake of PHBHHxPEG NPs, since a hydrophobic surface is known to disturb cell interaction. Yang et al. reported that the surface of PHA film demonstrated higher hydrophilicity and better cell compatibility after NaOH treatment . This can be explained by the ability of NaOH treatment to break down the ester bond of PHA backbone, leaving more hydroxyl group and carboxyl group on the surface of PHA film. Our previous study also indicated that the NaOH treatment increased the surface hydrophilicity of PHBHHx film and the neural stem cell-PHBHHx film interaction (data not published). The hydrophilic PEG represents a biocompatible material commonly used to enhance the biocompatibility of an object with good cell compatibility. Therefore, the emulsification/solvent evaporation method was used to expose PEG at the surface of PHBHHxPEG NPs and hence to increase the hydrophilicity of NPs surface as well as the cell-NPs interaction. In agreement, our results showed that cell contact was maximal in PHBHHxPEG NPs.
PEGylation of nanocomposites was reported to be able to resist nonspecific protein adsorption and have prolonged circulating half-life in vivo. However, in this study, the PHBHHxPEG NPs could not prevent the endocytosis by RAW264.7 murine macrophage-like cells. This might be explained by an insufficient PEG density on the colloidal surface of PHBHHxPEG NPs. PEG-modification of PLGA NPs is known to improve circulation time, depending on the molecular weight (chain length) and molar ratio (grafting efficiency) of PEG incorporation . After 5 min from administration, the remaining PLGA particles in circulation are about 5%, 25% and 50% for unmodified, PEG5000 modified and PEG20000 modified PLGA particles, respectively. This shows that the long PEG chain is necessary for increased anti-clearance properties. In our study, the PHBHHxPEG copolymer was synthesized by A. hydrophila by adding PEG200 in the culture medium. PEG200 attacks the carbonyl carbon of the PHBHHx chain directly and forms the end-capped PHBHHxPEG copolymer . Thus, in our experiments the incorporated PEG fragment was no longer than 3–4 units in each chain. While this was insufficient to promote the formation of a dense, hydrophilic cloud on the surface of NPs, potentially preventing macrophage-dependent opsonization, the use of PEG200 was sufficient to optimize NPs hydrophilicity and bioavailability.
Overall, this study represented the potential of PHBHHxPEG NPs as a promising kinase inhibitor delivery carrier in anti-cancer study. Our results indicated that the entrapment of rapamycin into PHBHHxPEG NPs could sufficiently enhance its bioavailability and anti-proliferation effect. Nonetheless, in vivo evaluation of circulating time and anti-proliferation ability of the rapamycin-loaded PHA NPs in animal models is still needed. Conversely, the proven effectiveness in cell based assays of this novel intracellular delivery nanocarrier opens the way to similar formulation of other kinase inhibitors. Since the PHBHHxPEG NPs based drug delivery carrier could also be internalized by other cell types such as macrophage, rapamycin-loaded PHBHHxPEG NPs might also have alternative applications, for example, in the field of immunosuppressant therapeutic tregimens.
Poly(3-hydroxybutyrate-co-3-hydroxyhexanoate) (PHBHHx) (Mw =4 × 105) was donated by Lab of Microbiology, Department of Biological Science and Biotechnology, Tsinghua University (Beijing, P. R. China). PHBHHxPEG (Mw =1.8 × 105) was produced by our group . Poly(vinyl alcohol) (PVA) (P1763), poly(DL-lactide) (PLA) (P1691) and rhodamine B (83689) were purchased from Sigma-Aldrich (USA). Rapamycin (S1039) was purchased from selleckchem (USA).
Preparation of drug-Loaded PHBHHx-PEG nanoparticles
The RAP-loaded NPs and rhodamine B-loaded NPs were fabricated by a modified emulsification/solvent evaporation method [8, 9, 21]. Briefly, 20 mg of polymers and RAP (2 mg) or rhodamine B (1 mg) were added into 1 ml chloroform and the mixture was stirred to ensure that all materials were dissolved. Then the polymer-drug organic solution was slowly dropped into 20 ml of 1% PVA (w/v) under sonication. The double emulsion was then deal with sonication using a probe sonicator (Sonics & Materials, Newtown, CT, USA) for 5 min, followed by moderately stirred with a magnetic mixer for 10 h to solidify the nano-droplets. Chloroform was removed by volatilization at room temperature. The NPs were collected by centrifugation at 12000 rpm for 30 min and then washed twice with phosphate buffered saline (PBS) solution. Three types of hydrophobic polymer NPs (PHBHHx, PHBHHxPEG and PLA) were prepared in this study.
Characterization of nanoparticles
The particle size distribution and polydispersity index (PDI) were measured by a laser light scattering machine (Zetasizer Nano ZS, Malvern, UK). The samples were diluted into proper concentration with deionized water and examined to determine the average particle diameters and PDI. The shape of resulting NPs was observed by JEM-2100 transmission electron microscope (JEOL Ltd. Japan).
Entrapment efficiency and drug-loading content measurement
Where Mi was the mass of RAP fed initially, Mt represented for the total amount of RAP in NPs and Mp was the mass of the resulting NPs, respectively . The amount of RAP was analyzed by high performance liquid chromatography (HPLC) with a SinoChrom ODS-BP column (5 μm, 4.6 mm × 15 mm; Elite Analytical Instruments, Dalian, P.R. China). To measure the amount of entrapped or retained RAP in NPs, 50 microliters of resuspended RAP-loaded NPs were dissolved in 450 μl acetonitrile at room temperature and then stored at 4°C for 4 hours to precipitate polymer. The supernatant was used to perform the HPLC analysis after filtrated with 0.2 μm filter.
In vitro drug release study
Cell culture and proliferation assay
Human prostate cancer cell line PC3 was used to evaluate the in vitro proliferation inhibition effect of RAP-loaded NPs. PC3 cells were maintained in RPMI 1640 (Invitrogen, USA) supplemented with 10% fetal bovine serum (Gibico) and 1% penicillin-streptomycin at 37°C in humidified environment of 5% CO2. The medium was replenished every other day and the cells were subcultured after reached confluence.
For measurement of proliferation, cells were seeded in triplicate at 2 × 103 cells/well in 96-well culture plates and incubated overnight to allow cell attachment. To evaluate the cytotoxicity of NPs, cells were treated with empty PHBHHx NPs and PHBHHxPEG NPs with the concentration of 100, 500 and 1000 μg/mL for 24 hours. Cells were incubated with the RAP-loaded PHBHHx NPs, PHBHHxPEG NPs or free RAP for 24 and 48 hours to analyze the anti-proliferation effects of RAP-loaded NPs on PC3 cell lines. Cell viability was quantified by a 3-(4,5-dimethylthiazol-2-yl)-2,5-diphenyltetrazolium bromide (MTT) assay. The absorbance of viable cells was measured at 570 nm using a microplate reader (Anthos 2020, Anthos Labtech Instruments, Wals., Austria). Relative cell viability was calculated with regard to that of the cell control at 24 hour, which was set to 100% viability.
Cellular uptake of nanoparticles
Human prostate cancer cell line PC3 and a murine macrophage cell line RAW264.7 cells were used to investigate the in vitro endocytosis of NPs. Cells were seeded in 96-well plates at 1 × 104 cells/well and incubated at 37°C with 5% CO2 in a humidified incubator overnight to allow cell attachment, followed by treating with rhodamine-loaded NPs (100 μg/mL) and free rhodamine B (with equal fluorescence intensity) of for 3 h. Medium was then discarded and cells were washed with PBS twice to remove the extracellular rhodamine B and rhodamine B-loaded NPs. New medium was added to each cell cultures again and PC3 and RAW264.7 cells were observed by fluorescence microscopy to evaluated cellular uptake of various NPs. The intracellular fluorescence intensities were quantified by fluorescence spectrophotometer (Infinite M200 PRO, Tecan Group Ltd. Switzerland).
mTOR inhibition assay and western blot analysis
Cells were seeded in 6-well plates at 2 × 105 cells/well and incubated at 37°C with 5% CO2 in a humidified incubator overnight to get attached and then treated with free RAP or RAP-loaded NPs for 24 h. After washing with cold PBS for two times, cells were lysated by adding RIPA lysis Buffer (50 mM Tris–HCl (pH 7.4), 150 mM NaCl, 1% NP-40), followed by incubating at 4°C for 30 min. Cell lysates were centrifuged at 10000 rpm for 5 min and supernatant was then loaded into 10% SDS–PAGE gels. After electrophoresis, proteins were transferred onto PVDF membranes, which were then blocked with 5% bovine serum albumin in TBST buffer for 1 h at room temperature. PVDF membranes were incubated overnight with an anti-phospho-p70S6 Kinase (Thr 389) antibody (Cell Signaling Technology Inc., USA, #9205), anti-p70S6 Kinase antibody (Cell Signaling Technology Inc., USA, #9202), anti-mTOR antibody (Cell Signaling Technology Inc., USA, #2972) and anti-β-actin antibody from Beijing Biosynthesis Biotechnology (Beijing, China), respectively, and subsequently hybridized with secondary HRP conjugated anti-rabbit IgGs (Zhongshan Goldenbridge Biotechnology, Beijing, China, #ZB-2301). The hybrid signals were detected by incubating with an enhanced chemiluminescence solution (ECL) purchased from Thermo scientific (#LK151361). The amount of phospho-p70S6K, total p70S6K, total mTOR and β-actin were analyzed by Quantity One software (Bio-Rad laboratory Inc., USA) and the relative phospho-p70S6K level was normalized according to the amount of total p70S6K.
All results were expressed as mean ± standard deviation of at least three independent experiments performed in triplicates. Statistical analysis was performed using a one-way analysis of variance (ANOVA) with Bonferroni post-hoctest. Differences were considered to be statistically significant at a level of p < 0.05.
Prof. Lu Shemin (College of Medicine, Xi’an Jiaotong University) is acknowledged for providing the murine macrophage cell line RAW264.7 cells. The authors would also like to express their thanks to Prof. Wu Daocheng and Prof. Liu Jiankang (both from School of Life Science and Technology, Xi’an Jiaotong University), for assistance with the characterization of nanoparticles and biological assay of mTOR inhibition, respectively. This work was supported by grants from the National Natural Science Foundation of China (81172170, 81371288), Science and Technology Research and Development Program of Shaanxi Province (2013KW32-04) and the Fundamental Research Funds for the Central Universities from Xi’an Jiaotong University.
- Kahan BD, Camardo JS: Rapamycin: clinical results and future opportunities. Transplantation. 2001, 72 (7): 1181-1193.View ArticleGoogle Scholar
- Meric-Bernstam F, Gonzalez-Angulo AM: Targeting the mTOR Signaling Network for Cancer Therapy. J Clin Oncol. 2009, 27 (13): 2278-2287.View ArticleGoogle Scholar
- Douros J, Suffness M: New Anti-Tumor Substances Of Natural Origin. Cancer Treat Rev. 1981, 8 (1): 63-87.View ArticleGoogle Scholar
- Simamora P, Alvarez JM, Yalkowsky SH: Solubilization of rapamycin. Int J Pharm. 2001, 213 (1–2): 25-29.View ArticleGoogle Scholar
- Dias VC, Yatscoff RW: An in vitro method for predicting in vivo oral bioavailability of novel immunosuppressive drugs. Clin Biochem. 1996, 29 (1): 43-49.View ArticleGoogle Scholar
- Chen GQ, Wu Q: The application of polyhydroxyalkanoates as tissue engineering materials. Biomaterials. 2005, 26 (33): 6565-6578.View ArticleGoogle Scholar
- Wu Q, Wang Y, Chen GQ: Medical application of microbial biopolyesters polyhydroxyalkanoates. Artif Cells Blood Substit Biotechnol. 2009, 37 (1): 1-12.View ArticleGoogle Scholar
- Lu XY, Ciraolo E, Stefenia R, Chen GQ, Zhang YL, Hirsch E: Sustained release of PI3K inhibitor from PHA nanoparticles and in vitro growth inhibition of cancer cell lines. Appl Microbiol Biotechnol. 2011, 89 (5): 1423-1433.View ArticleGoogle Scholar
- Xiong YC, Yao YC, Zhan XY, Chen GQ: Application of polyhydroxyalkanoates nanoparticles as intracellular sustained drug-release vectors. J Biomater Sci-Polym Ed. 2010, 21 (1): 127-140.View ArticleGoogle Scholar
- Zhang YL, Lu XY, Liu QQ, Li MC, Yang ZQ, Ma JG: Production and characterization of poly(3-hydroxybutyrate-co-3-hydroxyhexanoate)-poly(ethylene glycol) hybird copolymer with adjustable molecular weight. Chin J Polymer Sci. 2012, 30 (1): 101-111.View ArticleGoogle Scholar
- Blaser B, Waselle L, Dormond-Meuwly A, Dufour M, Roulin D, Demartines N, Dormond O: Antitumor activities of ATP-competitive inhibitors of mTOR in colon cancer cells. BMC Cancer. 2012, 12: 86-View ArticleGoogle Scholar
- Foster DA, Toschi A: Targeting mTOR with rapamycin: one dose does not fit all. Cell Cycle. 2009, 8 (7): 1026-1029.View ArticleGoogle Scholar
- Shi JJ, Votruba AR, Farokhzad OC, Langer R: Nanotechnology in Drug Delivery and Tissue Engineering: From Discovery to Applications. Nano Lett. 2010, 10 (9): 3223-3230.View ArticleGoogle Scholar
- Langer R: Drug delivery and targeting. Nature. 1998, 392 (6679): 5-10.Google Scholar
- Mora-Huertas CE, Fessi H, Elaissari A: Polymer-based nanocapsules for drug delivery. Int J Pharm. 2010, 385 (1–2): 113-142.View ArticleGoogle Scholar
- Wang M, Thanou M: Targeting nanoparticles to cancer. Pharmacol Res. 2010, 62 (2, Sp. Iss. SI): 90-99.View ArticleGoogle Scholar
- Yao YC, Zhan XY, Zhang J, Zou XH, Wang ZH, Xiong YC, Chen J, Chen GQ: A specific drug targeting system based on polyhydroxyalkanoate granule binding protein PhaP fused with targeted cell ligands. Biomaterials. 2008, 29 (36): 4823-4830.View ArticleGoogle Scholar
- Yang XS, Zhao K, Chen GQ: Effect of surface treatment on the biocompatibility of microbial polyhydroxyalkanoates. Biomaterials. 2002, 23 (5): 1391-1397.View ArticleGoogle Scholar
- van Vlerken LE, Vyas TK, Amiji MM: Poly(ethylene glycol)-modified nanocarriers for tumor-targeted and intracellular delivery. Pharm Res. 2007, 24 (8): 1405-1414.View ArticleGoogle Scholar
- Gref R, Minamitake Y, Peracchia MT, Trubetskoy V, Torchilin V, Langer R: Biodegradable Long-Circulating Polymeric Nanospheres. Science. 1994, 263 (5153): 1600-1603.View ArticleGoogle Scholar
- Perez C, Sanchez A, Putnam D, Ting D, Langer R, Alonso MJ: Poly(lactic acid)-poly(ethylene glycol) nanoparticles as new carriers for the delivery of plasmid DNA. J Control Release. 2001, 75 (1–2): 211-224.View ArticleGoogle Scholar
- Li Q, Wang Y, Feng NP, Fan ZZ, Sun J, Nan YL: Novel polymeric nanoparticles containing tanshinone IIA for the treatment of hepatoma. J Drug Target. 2008, 16 (10): 725-732.View ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an open access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.